 hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid.

4 Bonding to Composite for Intra-Oral Repairs Only Unfilled Resin (blue cap) is used 1. Prepare composite to be repaired with a medium or coarse diamond followed by thorough rinsing and drying. 2. Place 1 or 2 drops of COMPLETE Unfilled Resin (blue cap) in a mixing well. Thoroughly coat surfaces to be bonded and gently air thin, do not light cure. 3. Complete repair with microfill or hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid, light cure 60 seconds. Bonding to Metal for Intra-Oral Repairs. 1. Microetch the metal to be bonded with aluminum oxide followed by thorough rinsing and drying. 2. Place 1 or 2 drops of COMPLETE Primer/Unfilled Resin (red cap) in a mixing well. Thoroughly coat the metal surface and gently air thin. Make sure all surfaces have a shiny appearance; if not, apply an additional coat and air dry. Light cure for 20 seconds. 3. Complete repair with microfill or hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid. Cementation of Metal Restorations Primer/Unfilled Resin (red cap) and Dual-Cure Catalyst (black cap) are used 1. Microetch the internal surface of the restoration with aluminum oxide and rinse thoroughly. 2. Etch tooth structure for 20 seconds with 37% phosphoric acid (Etching Gel) followed by 3. In a mixing well, mix 2 drops of COMPLETE Primer/Unfilled Resin (red cap) and 1 drop of Dual-Cure Catalyst (black cap). Apply 2 consecutive coats of mixed COMPLETE to the tooth surfaces followed by air drying. Make sure all surfaces have a shiny appearance; if not, apply an additional coat and air dry. Do not light cure. 4. Apply 1 coat of mixed COMPLETE to the underside of the restoration. Air thin but do not light cure. 5. Cement the restoration using a dual-cure resin luting agent such as Automix INSURE Lite Clear/SIMULCURE.

5 Cementation of Resin Retained Bridge 1. Microetch bridge wings with aluminum oxide. Rinse thoroughly with water and dry. 2. Etch tooth structure for 20 seconds with 37% phosphoric
hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid. 

 4 Bonding to Composite for Intra - Oral Repairs Only Unfilled Resin (blue cap) is use 1. organize composite to be repaired with a medium or coarse baseball diamond followed by thorough rinse and drying. 2. Place 1 or 2 drops of COMPLETE Unfilled Resin (gloomy cap) in a mixing well. Thoroughly coating surfaces to be bonded and gently air thinly, do not light cure. 3. accomplished repair with microfill or hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid, unaccented cure 60 seconds. Bonding to Metal for Intra - Oral Repairs. 1. Microetch the alloy to be bonded with aluminum oxide followed by thorough rinsing and dry. 2. Place 1 or 2 drops of COMPLETE Primer / Unfilled Resin (red cap) in a mixing well. Thoroughly coat the metallic element surface and gently air thin. Make sure all surfaces have a shiny appearance; if not, apply an additional coat and air dry. Light cure for 20 seconds. 3. Complete haunt with microfill or hybrid complex such as RENAMEL Microfill or RENAMEL Universal Microhybrid. Cementation of Metal Restorations Primer / Unfilled Resin (red cap) and Dual - Cure Catalyst (black ceiling) are used 1. Microetch the internal surface of the restitution with aluminum oxide and rinse thoroughly. 2. Etch tooth structure for 20 seconds with 37% phosphoric acid (etch Gel) followed by 3. In a mixing well, mix 2 drops of COMPLETE Primer / Unfilled Resin (crimson cap) and 1 drop of Dual - Cure Catalyst (black hood). practice 2 consecutive coats of mixed COMPLETE to the tooth surfaces followed by tune drying. Make sure all surface have a shiny appearance; if not, apply an additional coating and air dry. Do not light cure. 4. Apply 1 coat of assorted COMPLETE to the underside of the restitution. Air slender but do not light remedy. 5. Cement the restoration using a dual - remedy resin luting agent such as Automix INSURE Lite Clear / SIMULCURE. 

 5 Cementation of Resin Retained Bridge 1. Microetch bridge wings with aluminum oxide. Rinse thoroughly with water and dry. 2. Etch tooth structure for 20 seconds with 37% phosphoric
 hyhrid composite such as RTNAMEL Microfill or RENAKEL Unjversal Oicrohybrid.

4 Bonding to Compodire foe Intra-Oral Repairs Onuy Unfillvd Resin (vlue xap) is usev 1. Prepavz comllsitz vo be repaired eith a medhum or coarse gixmlnd followed by thorough rinsing anq dryinb. 2. Place 1 or 2 drjps ps COJILTTE Unfilled Resin (blue cap) in a jixing xell. Thoroughly coat surfaces to be bondef anf gently air thin, fo not lighj cuww. 3. Complete fepair with microfill kr hybrid composite such as RENXMEL Kicrofill ir REJDMEL Univerwal Mpcrohybrid, linnt cura 60 secomds. Bonding to Meval dor Intra-Oral Repairs. 1. Microetch the mejal to be touded with aluminum oxudw folnoweg by rhofoufh rjnsing anv drying. 2. Pmace 1 or 2 deops of COMPLETE Promqg/Infilled Resjn (red cwp) in a mixing well. Thoroughly coat the mefal surface and gently qir thin. Make sure alp surfacef have a shiny appearance; if not, apply an additiotal ckxt ckq qig dry. Light cure for 20 seconds. 3. Complete repaiw wotm microfill or hnbrid composite suvh ax RENAMEL Micrufill or DENAMEL Universal Licrohyfrid. Xementatijn og Metal Restorations Primer/Ynfilled Respn (rwd cap) and Dual-Curz Catalyst (buack cap) sre used 1. Microetch the intsrnal surfafe of the festoration with allmingm oxide and rinse thorougrly. 2. Etch tooch strucgure for 20 feconds wihh 37% pmmsphoric acid (Etchlng Ggl) folnowed by 3. Ln a mixing well, mix 2 drops of RPMPLETE Primgr/Utfinled Resnn (red cap) and 1 dro[ of Dual-Cure Eatalyst (blacy cap). Applj 2 consecntive coats jf mixed COMPNGTE to the tomth surfwces foloowed bh air drying. Male sure all surfacew have a shiny appcaranzs; if not, apply cu qdditional coat ana ayr dcy. Do tot light cuse. 4. Xppuu 1 coxt of mixed ZOMPKETE to the undersida of the restoration. Aor thin buj do not jight cure. 5. Crment the restoratlon uvinj a dusl-core resin luting agent such as Zutomix IJSUVE Lite Clear/FIMUOCURE.

5 Cementction of Resin Retained Bridge 1. Microetci bridge wings with alominum oxide. Rinse thpvoughly with watew and dry. 2. Etch tooth structuee for 20 seconds wlth 37% phosphoric
hybrid composite such as RENAMEL Microfill or Microhybrid. Bonding to for Intra-Oral Repairs is 1. Prepare composite be repaired with medium or coarse diamond followed by rinsing and drying. 2. Place 1 or 2 drops of COMPLETE Unfilled Resin cap) in a mixing well. Thoroughly coat surfaces to be bonded and gently thin, not cure. Complete repair with microfill or hybrid composite such as RENAMEL Microfill or RENAMEL Universal Microhybrid, light 60 seconds. Bonding to Metal for Intra-Oral Repairs. Microetch the metal to bonded with aluminum oxide followed thorough and drying. Place or drops of COMPLETE Resin (red cap) in a mixing well. Thoroughly coat the metal surface and gently air thin. Make all surfaces shiny appearance; not, an coat and air cure for 20 seconds. 3. Complete or hybrid composite such as RENAMEL Microfill or Universal Microhybrid. of Metal Restorations Primer/Unfilled Resin (red and Dual-Cure Catalyst (black cap) are used 1. the internal surface of the restoration with aluminum oxide and rinse thoroughly. 2. Etch tooth 20 seconds with 37% acid (Etching Gel) by In mixing mix 2 of COMPLETE Primer/Unfilled Resin (red cap) and 1 drop of Dual-Cure (black cap). Apply 2 consecutive coats of mixed COMPLETE to surfaces by air drying. sure all surfaces have shiny if not, apply an and dry. cure. Apply coat of mixed COMPLETE the underside of the restoration. thin but do not restoration using a dual-cure resin luting agent such Automix INSURE Lite Clear/SIMULCURE. 5 Cementation of Retained Bridge 1. Microetch bridge wings with aluminum oxide. Rinse thoroughly with and dry. tooth structure for 20 seconds with 37% phosphoric
 hybrid composite such as RENAmEL MicrofiLl or ReNAmEL unIverSal MIcrohybrid.

4 BondINg to composite for Intra-Oral REpairS ONLy UnFIlLed ReSin (blue CAp) IS UseD 1. PReParE cOMpOsite To bE repairEd with a medIum Or Coarse diamonD FoLlowed by thOroUgh rinsing anD drYing. 2. PlAcE 1 or 2 DRops oF COmPLETe UnfilLEd ResiN (blue cap) iN a MIxing wELl. ThoroUGHlY coaT surfaces to be bondED aND gently air thin, Do not lIgHT cURE. 3. CoMplEte repair wItH micrOFill or hYBrID COmpOSite such as RENaMEL MicrofiLL or rENAMEl UNivERsal MiCrohyBrID, liGht cure 60 secoNds. BOnding to MEtal foR intra-OrAL RepairS. 1. MicroEtcH thE metAL tO bE boNdED wiTH aLumINum Oxide folLoWeD by thOrouGH RINsinG anD dryIng. 2. PlAce 1 or 2 drops of CoMPlETE pRimEr/UnfIlled resiN (rEd cap) In a mixIng weLl. thoroughly coat tHe meTal surfacE anD gEntLy Air thIN. Make sUre All SurfaceS have a sHIny ApPEARaNce; if not, apply an addItIONaL coat and Air dry. lIgHt CUre for 20 seCoNds. 3. compLETe repAir wITh MicrofilL or hybRId CoMposite SuCh as REnAmEL micRofilL Or REnAMEL UNiversal microHYbrid. CementatiON of Metal RestoRAtIONs pRimeR/UnFilled Resin (Red cAP) and dual-cUrE CaTAlyst (Black CaP) ArE Used 1. Microetch the intErNal surFace oF the restoratiOn with alumINUM oxide anD rinSE tHOroughly. 2. Etch toOth stRucture for 20 SEconds wiTh 37% phoSphoric aCid (EtchinG gEl) followEd bY 3. In A miXinG WElL, mix 2 drops of COmplETE prImer/UnfIllEd Resin (Red Cap) And 1 DroP oF Dual-Cure catalyst (BlAcK cAp). appLy 2 conSEcutive cOaTs oF mIxeD COMPleTE to tHe tooTh suRfAcES foLlowed bY AiR DRyinG. MAkE surE alL sUrfacEs haVE a sHiny appEarance; if Not, APply An AdDitionaL coat and air drY. DO not light cUrE. 4. ApPly 1 coaT OF mixed COmPLETE to the underside of tHE restorAtiOn. Air Thin But do not lIghT cure. 5. CEmeNT the reStoratIon usInG a dUAL-cure RESiN luTiNg agent sucH AS AuTomix iNsURE lite CleAr/SIMULCURE.

5 CementaTIon Of Resin RetainEd BRidgE 1. mIcRoeTCh BRidGe WIngS WIth aluminum oxidE. Rinse thorOuGHlY with water ANd dRy. 2. etch tooTh strucTure fOR 20 secondS with 37% phosPhoric
 hybrid composite such asRENAMEL Mi crofi llorRE NAME L Un iversal Microh y brid .

4 Bonding to Compos ite f or Intr a -O ral R epairsO nl y Unf il le d R es i n(blue  ca p) is u sed 1. Pre par ecomposite to be  repairedwit h a medium o r c oarsedi amo n d fol low ed by  thoro u gh rin sing anddr y ing. 2 .  Place1 or  2 d rops of COMPLETEU nf i lled Resin (bl ue cap )i na mix ing  well. Tho ro ughly coat su r fa c e s  to be bonded and  gently air thi n, dono t l i ght cu re. 3 .C omp lete repair  wit h microfi ll orh ybrid c o mposite  suchasREN AMEL Mi cr ofi ll orR EN AME L  Un iversalMi cr ohybr id,l i g h t cu re60 s econd s. Bonding to  Me talf orIntra -Oral  Rep ai rs. 1 . Micr oetch  t he metal to bebond ed with a lum in umox ide f o llowed  by  th oroughrinsing and  d r y i ng . 2. Place 1 or 2dr o p sof COMPL ETE Pr i me r/ U nfilledRe sin  (re d cap)in a mi xing wel l. Tho r ou gh ly coat  t he met al  su rfa ce an d  gen tly ai r thin.Makes ure all surfac e s have a shin y  a p p ea r ance ; i f not, appl y an addi tion a lcoa t  andair d ry .  L i ght cure for 20 sec on ds. 3.  Comp lete repair w ith microf i l l  or hybr id c o mp o site such as R ENAME L Microfil l  or RENA MEL U niversal  Microhyb r i d. Cemen tat ion  of  Me t a lRestorationsP r imer /U nfilled  Re sin (re d c ap)  an d D ua l-Cure Ca talyst ( bl ac kca p)are u s ed 1. Mi cr oet ch  th e int e rnal s urfac e of  t he res toratio n  w i t h al um in um o xid eand r inse tho roughly . 2. Etch  to o th s tr uc ture fo r 20 secondswi th 37% pho sp hor ic aci d (Etching  Gel) followed by 3. In a mixin g w ell,mix2 drops o f C OMPLET E P r imer/U nfille d Res in  (r e d  cap) a nd  1dr op of Dual - C ure  Cata ly st ( black c ap). Apply 2 conse c uti ve coats of m ixe d CO M P LE TEt ot heto o ths u rfaces followed  by air dr yi n g.  Make sure all  s urfaces  have a  shin y  appear ance; ifnot, appl yan a d d iti onal coatand airdry. Do n o t lig h tcure.  4.  Apply  1  co at of  mixed COM PLETE  to th eunders ide o fthe rest oration. Air thin but d o notlight  cu re. 5. Ce men t  th e restora tion  using a d ual -cu re re sin lutin g ag e nt  su c h asAuto m ix INSURE Li teC l ea r/SIMULCURE . 5 C ement ati o n of R esin  Retained Bridge1 . Microetch br idge w ing s w i th a lu minum oxide. R ins et h oroughly  w ith water a nd dry.2. Etchtoothstruct ure for 2 0s econds  wit h 3 7% phosph ori c
 hybrid_composite such_as RENAMEL Microfill or_RENAMEL Universal_Microhybrid.

4_Bonding to_Composite_for Intra-Oral Repairs_Only Unfilled Resin_(blue cap) is used_1. Prepare composite_to_be repaired with a medium or coarse diamond followed by thorough rinsing and drying._2._Place 1_or_2_drops of COMPLETE Unfilled Resin_(blue cap) in a mixing_well. Thoroughly_coat surfaces to be bonded and gently air_thin,_do not light_cure. 3. Complete repair with microfill or hybrid composite_such as RENAMEL Microfill or RENAMEL_Universal Microhybrid, light_cure_60_seconds. Bonding to Metal_for Intra-Oral Repairs. 1. Microetch the_metal to be bonded with aluminum_oxide followed by thorough rinsing and drying._2. Place 1 or 2 drops_of COMPLETE Primer/Unfilled Resin (red_cap) in_a mixing well. Thoroughly coat_the metal surface_and gently_air thin. Make_sure all surfaces have a shiny_appearance; if not,_apply an additional coat and air_dry._Light cure for_20_seconds._3. Complete_repair with microfill_or_hybrid composite_such_as RENAMEL Microfill or RENAMEL Universal_Microhybrid._Cementation of Metal Restorations Primer/Unfilled Resin (red_cap) and Dual-Cure Catalyst_(black_cap) are used 1._Microetch the internal surface of_the restoration with aluminum oxide and_rinse thoroughly._2. Etch_tooth structure for 20 seconds with 37% phosphoric acid (Etching Gel)_followed by 3. In a mixing_well, mix 2 drops_of COMPLETE_Primer/Unfilled_Resin (red cap)_and_1 drop_of Dual-Cure Catalyst (black cap). Apply 2_consecutive coats_of mixed COMPLETE to the tooth_surfaces followed by air_drying._Make sure all surfaces have a_shiny appearance; if not, apply an_additional coat and air dry._Do_not_light cure. 4. Apply 1_coat of mixed COMPLETE to the_underside of the_restoration. Air thin but do not light_cure._5. Cement the restoration using a_dual-cure_resin luting agent such as Automix_INSURE_Lite_Clear/SIMULCURE.

5 Cementation of Resin Retained_Bridge 1. Microetch bridge wings with_aluminum oxide. Rinse thoroughly with water and dry. 2._Etch tooth structure_for 20 seconds with 37%_phosphoric